期号 
Int. J. Simul. Multidisci. Des. Optim.
卷号 12, 2021
Computation Challenges for engineering problems



文献编号  10  
页数  8  
DOI  https://doi.org/10.1051/smdo/2021012  
网上发表时间  2021年7月22日 
Research Article
Design and simulation of multilayer hybrid foam material for acoustic application
^{1}
Department of Automobile Engineering, Acharya Institute of Technology, Bangalore, India
^{2}
School of Mechanical and Building Sciences, Vellore Institute of Technology, Chennai 600127, India
^{3}
Electric Vehicles Incubation, Testing and Research Centre, Vellore Institute of Technology Chennai, India
^{4}
Swinburne University of Technology Sarawak Campus, Malaysia
^{*} email: mechanicalyuva5236@gmail.com
Received:
10
January
2021
Accepted:
7
July
2021
New acoustic multilayer absorber fabricated by coupling closedcell metallic foam and opencell polymeric foam, which aimed to develop a practical use of metallic foam in the noise control application. In prior, the individual sound absorption coefficient of both foam materials with different thicknesses measured by the impedance tube method as per ASTM E1050. Using inverse characterization technique, the intrinsic properties needed for five parameter models in a numerical study are predicted. The measured characteristic impedance, complex wave propagation, and sound absorption coefficient of the individual foams are in close agreement with the prediction. Subsequently, a different configuration of multilayer absorber is modeled using obtained properties, and their acoustic performance is evaluated. The result indicates that the coupling of polymeric foam with metallic one exhibits enhanced sound absorption and usage of closedcell metallic foam in noise control material. Furthermore, the result demonstrates that absorption capability entirely relies on the placement of polymeric foam in the configuration. The proposed hybrid multilayer absorber coupled with test bench car for interior acoustic study, where 5–30 dB is reduction is noticed in 1/3rd octave plot.
Key words: Aluminium foam / polymeric foam / sound absorption / particle swarm optimization / test bench car
© L. Yuvaraj et al., Published by EDP Sciences, 2021
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (https://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
1 Introduction
Lightweight foamed materials are produced from ceramics, metals, and polymers, used in many engineering applications due to high energy absorption and strength to weight ratio. Based on the connectivity between the cells, the foam can be classified into an opencell and a closedcell. Mostly the aluminum foam that is available in commercial is closed cell foam. The sound absorption characteristic of closedcell foam is good only at higher frequency regions [1]. The main reason is that the metallic frame is stiffer than the surrounding fluid, so the acoustic losses viscous and thermal occur at metalfluid interface limited by isolated closed cells. Also, it depends on the closed pore size, shape, and structure. Extensive research was carried out in polymeric foam, which is fully reticulated, partially reticulated, and completely closed to obtain the acoustic properties [2–4]. These materials have a wide range of acoustic properties depending on poroelastic nature, pore size, and reticulation rate. Sound absorption of opencell and partial reticulated foam exhibits good viscous and thermal losses effect.To overcome the drawback of aluminium foam, Sound absorption of highdensity material can be enhanced by the combination of lowdensity material as a multilayer porous material [5] which acts as a massspring system leads to additional attenuation of sound.
Two critically linked membranetype acoustic metamaterials sandwiching a porous material layer were proposed by Wang et al. [6] as a layered porous material. Adaptive algorithms are used to detect the radiating source which is not familiar with weighted classical array of sensors [7]. The study reported that the material characterization is used to design resonator by optimization process [8]. Also, that the nonacoustic parameter needed for numerical simulation can be predicted using inverse characterisation with different algorithm for instance particle swarm optimization algorithm (PSO) [9], genetic algorithm [10] and so on. The sound absorption coefficient, especially the low frequency sound absorption coefficient is increased obviously as the growing of samples thickness. This phenomenon can be found in porous metal as well as flexible materials. The detailed finite element modeling presented in various studies by author and referred [10–12]. The present work demonstrates closedcell metallic foam usage in the acoustic application by proposing new hybrid foam comprises closed cell metallic foam and opencell polymeric foam as a multilayer porous absorber. The proposed configuration experimented in impedance tube and same is validated by numerical results. Furthermore, the best configuration is coupled with test bench car to evaluate sound pressure level using COMSOL multiphysics acoustic module.
2 Materials and methods
2.1 Aluminum foam
The metallic aluminium (Al) foam procured from local source whose dimension ranges 0.1 × 0.1 × 0.01 mm^{3} and cutted into impedance diameter 96 mm. The properties of Al foam depicted in Table 1.
Properties of Al foam.
Foam preparation specification.
2.2 Polyurethane foam
Flexible polyurethane is synthesized by isocyanate and polyol, and those chemicals duly supplied Manali Petrochemicals Limited (Chennai, India). EMPEYOL WSF 300/1–8(HLD) used as a polyol, which is a premixture of all additives like a catalyst, stabilizer, water, chain extender, surfactants, and WANNATE 8018 as isocyanate. The properties of foam chemicals given in Table 2.
2.3 Hybrid foam
Once the sample cut into the desired shape, placed in a circular die, and the polyol isocyanate mixture is poured. After the demould time, the sample is taken out to remove the additional thickness material also the rough surface of aluminum foam, making a strong bond when the molten polyol mixture cures. The prepared sample and its configuration is shown in Figures 1 and 2. The overall thickness of all configurations is 40 mm is maintained, and the sample name is given in the following ways as depicted in Table 3.
Fig. 1 Prepared hybrid foam. 
Fig. 2 Schematic diagram of a multilayer configuration. 
Sample nomenclature.
2.4 Experimental testing
The sound absorption coefficient of the individual sample and hybrid foam is tested in impedance as per ASTM E 1050 [13], where the frequency range of interest is 220 Hz to 4000 Hz. Samples are cut into circular sections with a diameter of 33 and 100 mm. Three samples for each category are used for this test. The white noise signal excited from sourcechannel DAQ connected to the power amplifier then to 16 Ω speakers at one end and two 1/2″ MicrotechGefell microphones connected to M+P Vibpilot DAQ. Using the M+P spectrum analyzer, the time domain was extracted of useful bandwidth 8196 Hz with a frequency resolution of 0.5 Hz, which is imported to MATLAB® to calculate transfer function between two microphones. The schematic diagram of the impedance tube is shown in Figure 3.(1)where K_{0} the wavenumber, f is the frequency, and C_{0} is the speed of sound(2)where H_{12} is the acoustic transfer function, p_{1} and p_{2} are the measured acoustic pressure of the two microphones, and x_{1} and x_{2} are the distance between the reference plane (sample position of x = 0) and the two microphones. Finally, the reflection coefficient and sound absorption coefficient α is obtained by(3) (4)
Fig. 3 Schematic diagram of impedance tube. 
2.5 Inverse characterization using PSO
The PSO works on the social sharing of information of organism among the fish in a flock. While moving into the community, fish exchange information about theirposition, velocity, and fitness function value. In the PSO algorithm, the words fish andparticle are used interchangeably. Individual particle provides information about itsposition vector in the solution space and the associated velocity vector. All particleschange their position at a particular time set in the algorithm. Then the velocity vector data isused to calculate the new location for the next time step. The PSO algorithmrecords the information about the best individual position attained by each particle known as p^{best} and the best global position achieved by all particles together knownas G^{best}. In each iteration, G^{best} represents a least error with the measured value and all p^{best} values follow G^{best} values to give the best solution. Hence, with the knowledge of these two best values, all particles collectively move towards the optimum globalposition.In this optimization problem, the design variables are the nonacousticalparameters. The nonacoustical parameters for the JohnsonChampouxAllard (JCA) equivalent fluid modelwith a rigid frame model are porosity, Tortuosity, flow resistivity, viscous characteristic length (VCL), and thermal characteristic length (TCL). The objective function used here is defined by equation (5) (5)where E (α) is the normalised means square error, n is the total number of data, is the experimental sound absorption, is the predicted sound absorption using JCA model. Constraints used for this study presented in Table 4.
Constraint for the design variable.
2.6 Numerical simulation
2.6.1 Multilayer simulation
Sound absorption of multilayer configuration of hybrid foam analyzed numerically using COMSOL Multiphysics [7–9]. In component section, using the geometry option, a block created and the plane partitioned into 5 domains with the help of Boolean operation. The lengthier domain chosen as pressure acoustics module and air material property is applied. Similarly, four equal thicknesses are chosen poroelastic waves module and material property used as per configuration order. Multiphysics coupling is applied to make the interaction between porous and acoustic boundary layers. Hexahedron element mapped for the whole model and size of the component is chosen based on six elements per wavelength on a higher frequency. For excitation plane wave radiation with unit Pascal is applied. Figure 4 presents the geometry model, mesh model, and simulated model. The material property used for simulation is depicted in Table 5.
Fig. 4 Numerical simulation of fourlayer hybrid foam. 
Predicted nonacoustic parameters using PSO algorithm.
2.6.2 Test bench car simulation
To examine the effect of the proposed hybrid foam in the car interior, a test bench car simulation was carried out in COMSOL Multiphysics. The dimensions of the test bench car are length × height × depth is 3.0 m × 1.4 m × 1.7 m,and the windshield has its lower end 0.8 m above the floor and with an inclination of 32° such that the entire volume of the geometry is 6.5 m^{3}. The given dimension resembles the actual car and part body for instance the section which separates engine compartment and cabin is modeled as proposed material because engine noise major source of noise. Based on this front section, hybrid foam is modeled, and better configuration material is applied. A monopole point flow source of strength Q_{S} = 10^{−5} m^{3}/s located at the point P_{0} = (0.21, 0, and 1.28) is chosen. Pressure acoustic frequency domain module applied to the entire model and hybrid foam defined as poroacoustic material, and five parameter JCA model was chosen from dropdown. The model has meshed with Physics controlled free triangular element with fine size, and the study conducted over the frequency range of 1001000 Hz. The sound pressure level measured at the point P_{1} = (1.34, 1.22, and 0.8), geometry model, and SPL simulation is shown in Figures 5 and 6 respectively.
Fig. 5 Design of test bench car coupled with hybrid foam. 
Fig. 6 Numerical simulation of test bench car coupled with hybrid foam. 
3 Results and discussion
3.1 Experimental sound absorption result
Figure 7 represents the prepared multilayer configuration's experimental sound absorption coefficient; the metallic foam sample of 40 mm possesses good sound absorption only at a higher frequency region. This is due to limited viscous losses that too only on the surface of Al foam, which means higher resistance to the propagation of sound offered by the material. For sample, PU 40 foam sample open cell in nature also exhibits poroelastic property, so the viscous and thermal losses will be comparatively high compared to AL 40, leading to better sound absorption. To enhance sound absorption, this study attempt to produce combination material in a multilayer configuration. 20 mm Al foam kept as face layer followed that 20 mm PU foam added as an additional layer, now the total configuration AL20PU20 is maintained as 40 mm thickness. From the tested result, we can notice that sound absorption is slightly resonant behavior and much better than the AL40 sample, also roughly near to the performance of PU40. This is caused by highdensity AL20 material acting as mass and low density PU20 act as spring, so the whole configuration possesses additional dampening. By reversing the sample now the configuration is PU20AL20, and its corresponding result indicates that the sound absorption starts well in the lowfrequency region near 500 Hz. The possible reason for this improved sound absorption is low frequency has higher energy, so when it crosses the PU20, half of the sound energy is attenuated, and the rest is reacted with AL20. Further, the configuration is designed with four layers, each value a thickness of 10mm; now, the sample configuration is ALPUALPU, which resembles the double springmass system. Because of this effect, the resonant behavior is identified from the absorption plot, also the peak sound absorption places in the lowfrequency region. After reversing the sample now the configuration PUALPUAL is posses better sound absorption among all, the peak sound absorption placed in below 500 Hz, the sound energy attenuated by each layer. Figure 8 represents the validation plot of experimental and numerical results of all samples that possess fair agreement.
Fig. 7 Results of experimental sound absorption. 
Fig. 8 Validation results of experimental and numerical sound absorption (a) AL 40, (b) PU 40, (c) AL20PU20, (d) PU20AL20, (e) ALPUALPU, (f) PUALPUAL. 
3.2 Test bench car analysis result
For a simple case study, the better performing configuration sample PUALPUAL corresponding predicted values are used to model the hybrid foam and couple to test bench car for interior acoustic simulation. The numerical results of test bench simulation with and without hybrid foam are plotted in Figure 9. From the results, it is understood that the proposed configuration suppresses the majority of dominant modes. Further indepth outlook the result plotted in 1/3rd octave band in Figure 10, which is mainly used in environmental and noise control application. The octave plots show 5–30 dB reduction in SPL inside the car cavity.
Fig. 9 Result comparison of test bench car with and without hybrid material. 
Fig. 10 SPL comparison plot in 1/3rd octave plot. 
4 Conclusion
The hybrid foam was fabricated by developing a multilayer configuration from Al (closed cell) and PU (open cell) foam. The measured sound absorption of different layer configurations used to predict the nonacoustic parameters using the PSO algorithm. A simplified numerical model developed in COMSOL Multiphysics to evaluate sound absorption from the predicted parameters. The sound absorption coefficient of the experimental and numerical results are in good agreement. Further, the combination of opencell and closedcell foam enhances the sound absorption in a wide range of frequency. Significantly, the 10 mm layer configuration exhibits better acoustic performance than the 20 and 40 mm configuration. Once the optimum performed design is identified and its corresponding predicted value used to model the poroacoustic material to perform interior acoustic analysis. The sound pressure level of test bench car analysis is compared with and without hybrid foam material. From the numerical results the proposed configuration is capable of noise reduction of 5–30 dB in 1/3rd octave band.
References
 N. Dukhan, Metal Foams: Fundamentals and Applications, DEStech Publications, Inc. (2013) [Google Scholar]
 J.P. Arenas, M.J. Crocker, Recent trends in porous soundabsorbing materials, Sound Vibr. 44, 12–18 (2010) [Google Scholar]
 N. Kino, G. Nakano, Y. Suzuki, Nonacoustical and acoustical properties of reticulated and partially reticulated polyurethane foams, Appl. Acoust. 73, 95–108 (2012) [Google Scholar]
 O. Doutres, N. Atalla, K. Dong, A semiphenomenological model to predict the acoustic behavior of fully and partially reticulated polyurethane foams, J. Appl. Phys. 113, 054901 (2013) [CrossRef] [Google Scholar]
 L. Yuvaraj, S. Jeyanthi, Acoustic performance of countersunk microperforated panel in multilayer porous material, Build. Acoust. 27, 3–20 (2020) [Google Scholar]
 X. Wang, X. Luo, H. Zhao, Z. Huang, Acoustic perfect absorption and broadband insulation achieved by doublezero metamaterials, Appl. Phys. Lett. 112, 021901 (2018) [Google Scholar]
 J. Lardiès, H. Ma, M. Berthillier, Localization of radiating sources by an acoustical array, Int. J. Simul. Multidiscip. Des. Optim. 4, 135–140 (2010) [Google Scholar]
 P. Salzenstein, An example of design, optimization, stabilization and noise performances of resonatorbased optoelectronic oscillators, Int. J. Simul. Multidiscip. Des. Optim. 10, A2 (2019) [CrossRef] [Google Scholar]
 P.V. Bansod, A.R. Mohanty, Inverse acoustical characterization of natural jute sound absorbing material by the particle swarm optimization method, Appl. Acoust. 112, 41–52 (2016) [Google Scholar]
 L. Yuvaraj, S. Jeyanthi, A. Yogananda, An acoustical investigation of partial perforation in jute fiber composite panel, Mater. Today: Proc. (2020) [Google Scholar]
 L. Yuvaraj, S. Jeyanthi, L.B. MailanChinnapandi, Experimental and finite element approach for finding sound absorption coefficient of biobased foam, J. Vibroeng. 21, 1761–1771 (2019) [Google Scholar]
 R. Sailesh, L. Yuvaraj, J. Pitchaimani, M. Doddamani, L.B.M. Chinnapandi, Acoustic behaviour of 3D printed biodegradable microperforated panels with varying perforation crosssections, Appl. Acoustics 174, 107769 (2021) [Google Scholar]
 ASTM Standard E105012, Standard test method for impedance and absorption of acoustical materials using a tube, two microphones, and a digital frequency analysis system [Google Scholar]
Cite this article as: L. Yuvaraj, S. Jeyanthi, Lenin Babu Mailan Chinnapandi, Elammaran Jayamani, Design and simulation of multilayer hybrid foam material for acoustic application, Int. J. Simul. Multidisci. Des. Optim. 12, 10 (2021)
All Tables
All Figures
Fig. 1 Prepared hybrid foam. 

In the text 
Fig. 2 Schematic diagram of a multilayer configuration. 

In the text 
Fig. 3 Schematic diagram of impedance tube. 

In the text 
Fig. 4 Numerical simulation of fourlayer hybrid foam. 

In the text 
Fig. 5 Design of test bench car coupled with hybrid foam. 

In the text 
Fig. 6 Numerical simulation of test bench car coupled with hybrid foam. 

In the text 
Fig. 7 Results of experimental sound absorption. 

In the text 
Fig. 8 Validation results of experimental and numerical sound absorption (a) AL 40, (b) PU 40, (c) AL20PU20, (d) PU20AL20, (e) ALPUALPU, (f) PUALPUAL. 

In the text 
Fig. 9 Result comparison of test bench car with and without hybrid material. 

In the text 
Fig. 10 SPL comparison plot in 1/3rd octave plot. 

In the text 
Current usage metrics show cumulative count of Article Views (fulltext article views including HTML views, PDF and ePub downloads, according to the available data) and Abstracts Views on Vision4Press platform.
Data correspond to usage on the plateform after 2015. The current usage metrics is available 4896 hours after online publication and is updated daily on week days.
Initial download of the metrics may take a while.